Handbook of Damage Mechanics pp 1-24 | Cite as

# Healing, Super Healing, and Other Issues in Continuum Damage Mechanics

## Abstract

In this chapter, after a quick introduction on the literature of healing and super healing concept, the damage/healing mechanics principles are investigated. The concept of super healing of materials is then introduced into the framework of continuum damage mechanics (CDM). Super-healed material can be seen as a strengthened material by further healing when the whole damage is recovered by healing of a damaged material. Therefore, in this chapter the process of healing beyond what is necessary for damage recovery is called super healing. Super material is the final objective of the super healing process when the material achieves more stiffness at the end of super healing process. Then, by introducing the anisotropic super healing concept, these concepts are generalized in tensorial form to be used in anisotropic damage and healing of materials. Consequently, three fundamental issues in CDM are discussed. Nature of the damage process is investigated by dissecting the expression of the effective stress into an infinite geometric series. Several stages of damage are introduced which are termed primary, secondary, tertiary, etc., using this expression. New definition of the damage variable is then introduced for small damage cases. The new concept of undamageable materials that maintain a zero value of the damage variable throughout the deformation process is introduced. Finally and in the last section of the chapter, the forming of a singularity which leads to initiation of the process of fracture is shown in a continuous region within the framework of CDM. The internal damage processes leading to a singularity are illustrated mathematically. This section potentially provides a crucial link between the damage and fracture mechanics.

### Keywords

Fatigue Rubber Clarification### References

- J.A. Adam, A simplified model of wound healing (with particular reference to the critical size defect). Math. Comput. Model.
**30**, 23–32 (1999)CrossRefMathSciNetGoogle Scholar - E.M. Arruda, M.C. Boyce, A three-dimensional constitutive model for the large stretch behavior of rubber elastic materials. J. Mech. Phys. Solids
**41**, 389–412 (1993)CrossRefGoogle Scholar - E.J. Barbero, F. Greco, P. Lonetti, Continuum damage-healing mechanics with application to self-healing composites. Int. J. Damage Mech.
**14**, 51–81 (2005)CrossRefGoogle Scholar - A.F. Bower,
*Applied Mechanics of Solids*(CRC press, Boca Raton, 2011)Google Scholar - A. Cauvin, R.B. Testa, Damage mechanics : basic variables in continuum theories. Int. J. Solids Struct.
**36**, 747–761 (1999)CrossRefMATHMathSciNetGoogle Scholar - J.L. Chaboche, On some modifications of kinematic hardening to improve the description of ratchetting effects. Int. J. Plast.
**7**, 661–678 (1991)CrossRefGoogle Scholar - J.L. Chaboche, Thermodynamic formulation of constitutive equations and application to the viscoplasticity and viscoelasticity of metals and polymers. Int. J. Solids Struct.
**34**, 2239–2254 (1997)CrossRefMATHGoogle Scholar - C.L. Chow, M. Jie, Anisotropic damage-coupled sheet metal forming limit analysis. Int. J. Damage Mech.
**18**, 371–392 (2009)CrossRefGoogle Scholar - C. Chow, J. Wang, An anisotropic theory of elasticity for continuum damage mechanics. Int. J. Fract.
**33**, 3–16 (1987)CrossRefGoogle Scholar - W.L. George, J.A. Warren, A parallel 3D dendritic growth simulator using the phase-field method. J. Comput. Phys.
**177**, 264–283 (2002)CrossRefMATHGoogle Scholar - V. Ginzburg, On the theory of superconductivity. Il Nuovo Cimento (1955–1965)
**2**, 1234–1250 (1955)CrossRefMATHGoogle Scholar - V. Ginzburg, L.D. Landau, On the theory of superconductivity. Zh. Eksp. Teor. Fiz.
**20**(1950), 1064–1082 (1965). Translation in Collected papers of L.D.Landau. Pergamon, OxfordGoogle Scholar - L. Gránásy, T. Börzsönyi, T. Pusztai, Nucleation and bulk crystallization in binary phase field theory. Phys. Rev. Lett.
**88**, 206105 (2002)CrossRefGoogle Scholar - N.R. Hansen, H.L. Schreyer, A thermodynamically consistent framework for theories of elastoplasticity coupled with damage. Int. J. Solids Struct.
**31**, 359–389 (1994)CrossRefMATHGoogle Scholar - M. John, G. Li, Self-healing of sandwich structures with grid stiffened shape memory polymer syntactic foam core. Smart Mater. Struct.
**19**, 1–12 (2010)Google Scholar - L.M. Kachanov, On the creep fracture time. Izv Akad. Nauk USSR Otd. Tekh.
**8**, 26–31 (1958)Google Scholar - P.I. Kattan, G.Z. Voyiadjis, A plasticity-damage theory for large deformation of solids—II. Applications to finite simple shear. Int. J. Eng. Sci.
**31**, 183–199 (1993)CrossRefMATHGoogle Scholar - P.I. Kattan, G.Z. Voyiadjis, Decomposition of damage tensor in continuum damage mechanics. J. Eng. Mech.
**127**, 940–944 (2001)CrossRefGoogle Scholar - R. Kobayashi, Simulations of three dimensional dendrites, in
*Pattern Formation in Complex Dissipative Systems*, ed. by S. Kai (World Scientific, Singapore, 1992), pp. 121–128Google Scholar - L.D. Landau, D. Ter Haar,
*Collected Papers of LD Landau*(Pergamon Press, Oxford, 1965)Google Scholar - H. Lee, K. Peng, J. Wang, An anisotropic damage criterion for deformation instability and its application to forming limit analysis of metal plates. Eng. Fract. Mech.
**21**, 1031–1054 (1985)CrossRefGoogle Scholar - J. Lemaitre, How to use damage mechanics. Nucl. Eng. Des.
**80**, 233–245 (1984)CrossRefGoogle Scholar - J. Lemaitre, Coupled elasto-plasticity and damage constitutive equations. Comput. Methods Appl. Mech. Eng.
**51**, 31–49 (1985)CrossRefMATHGoogle Scholar - J. Lemaitre, J.L. Chaboche,
*Mechanics of Solid Materials*(Cambridge University Press, Cambridge, 1990)CrossRefMATHGoogle Scholar - G. Li, M. John, A self-healing smart syntactic foam under multiple impacts. Compos. Sci. Technol.
**68**, 3337–3343 (2008)CrossRefGoogle Scholar - G. Li, V.D. Muthyala, Impact characterization of sandwich structures with an integrated orthogrid stiffened syntactic foam core. Compos. Sci. Technol.
**68**, 2078 (2008)CrossRefGoogle Scholar - G. Li, D. Nettles, Thermomechanical characterization of a shape memory polymer based self-repairing syntactic foam. Polymer
**51**, 755–762 (2010)CrossRefGoogle Scholar - G. Li, N. Uppu, Shape memory polymer based self-healing syntactic foam: 3-D confined thermomechanical characterization. Compos. Sci. Technol.
**70**, 1419–1427 (2010)CrossRefGoogle Scholar - Y.L. Liu, Y.W. Chen, Thermally reversible cross-linked polyamides with high toughness and self-repairing ability from maleimide- and furan-functionalized aromatic polyamides. Macromol. Chem. Phys.
**208**, 224–232 (2007)CrossRefGoogle Scholar - I. Loginova, G. Amberg, J. Ågren, Phase-field simulations of non-isothermal binary alloy solidification. Acta Mater.
**49**, 573–581 (2001)CrossRefGoogle Scholar - V.A. Lubarda, D. Krajcinovic, Damage tensors and the crack density distribution. Int. J. Solids Struct.
**30**, 2859–2877 (1993)CrossRefMATHGoogle Scholar - S. Miao, M.L. Wang, H.L. Schreyer, Constitutive models for healing of materials with application to compaction of crushed rock salt. J. Eng. Mech.
**121**, 1122–1129 (1995)CrossRefGoogle Scholar - S. Murakami, Notion of continuum damage mechanics and its application to anisotropic creep damage theory. ASME Trans. J. Eng. Mater. Technol.
**105**, 99–105 (1983)CrossRefGoogle Scholar - B. Murray, A. Wheeler, M. Glicksman, Simulations of experimentally observed dendritic growth behavior using a phase-field model. J. Cryst. Growth
**154**, 386–400 (1995)CrossRefGoogle Scholar - M. Naderi, A. Kahirdeh, M. Khonsari, Dissipated thermal energy and damage evolution of Glass/Epoxy using infrared thermography and acoustic emission. Compos. Part B
**43**, 1613–1620 (2012)CrossRefGoogle Scholar - S. Nemat-Nasser, Decomposition of strain measures and their rates in finite deformation elastoplasticity. Int. J. Solids Struct.
**15**, 155–166 (1979)CrossRefMATHGoogle Scholar - S. Nemat-Nasser,
*On Finite Plastic Flow of Crystalline Solids and Geomaterials*(DTIC Document, Fort Belvoir, 1983)Google Scholar - J. Nji, G. Li, A self-healing 3D woven fabric reinforced shape memory polymer composite for impact mitigation. Smart Mater. Struct.
**19**, 1–9 (2010a)CrossRefGoogle Scholar - J. Nji, G. Li, A biomimic shape memory polymer based self-healing particulate composite. Polymer
**51**, 6021–6029 (2010b)CrossRefGoogle Scholar - J.W.C. Pang, I.P. Bond, A hollow fibre reinforced polymer composite encompassing self-healing and enhanced damage visibility. Compos. Sci. Technol.
**65**, 1791–1799 (2005)CrossRefGoogle Scholar - T. Park, G. Voyiadjis, Kinematic description of damage. J. Appl. Mech.
**65**, 93–98 (1998)CrossRefGoogle Scholar - R. Pavan, B. Oliveira, S. Maghous, G. Creus, A model for anisotropic viscoelastic damage in composites. Compos. Struct.
**92**, 1223–1228 (2010)CrossRefGoogle Scholar - Y.N. Rabotnov, Paper 68: on the equation of state of creep, in
*Proceedings of the Institution of Mechanical Engineers, Conference Proceedings*, SAGE Publications, 1963, pp. 2–117, 112–122Google Scholar - Y.N. Rabotnov, Creep rupture, in
*Proceedings of the XII International Congress on Applied Mechanics*, 1968, pp. 342–349Google Scholar - F. Sidoroff, Description of anisotropic damage application to elasticity, in
*Proceedings of the IUTAM Colloquium on Physical Nonlinearities in Structural Analysis*, Berlin, 1981, pp. 237–244Google Scholar - A.H.R.W. Simpson, T.N. Gardner, M. Evans, J. Kenwright, Stiffness, strength and healing assessment in different bone fractures – a simple mathematical model. Injury
**31**, 777–781 (2000)CrossRefGoogle Scholar - I. Singer-Loginova, H. Singer, The phase field technique for modeling multiphase materials. Rep. Prog. Phys.
**71**, 106501 (2008)CrossRefGoogle Scholar - K.S. Toohey, N.R. Sottos, J.A. Lewis, J.S. Moore, S.R. White, Self-healing materials with microvascular networks. Nat. Mater.
**6**, 581–585 (2007)CrossRefGoogle Scholar - J.D. van der Waals, The thermodynamic theory of capillarity under the hypothesis of a continuous variation of density. J. Stat. Phys.
**20**, 200–244 (1979)CrossRefGoogle Scholar - R.J. Varley, S. van der Zwaag, Towards an understanding of thermally activated self-healing of an ionomer system during ballistic penetration. Acta Mater.
**56**, 5737–5750 (2008)CrossRefGoogle Scholar - G.Z. Voyiadjis, Degradation of elastic modulus in elastoplastic coupling with finite strains. Int. J. Plast.
**4**, 335–353 (1988)CrossRefGoogle Scholar - G.Z. Voyiadjis, P.I. Kattan, A coupled theory of damage mechanics and finite strain elasto-plasticity—II. Damage and finite strain plasticity. Int. J. Eng. Sci.
**28**, 505–524 (1990)CrossRefMATHGoogle Scholar - G.Z. Voyiadjis, P.I. Kattan, A plasticity-damage theory for large deformation of solids—I. Theoretical formulation. Int. J. Eng. Sci.
**30**, 1089–1108 (1992)CrossRefMATHGoogle Scholar - G.Z. Voyiadjis, P.I. Kattan,
*Damage Mechanics*(CRC, Boca Raton, 2005)CrossRefMATHGoogle Scholar - G.Z. Voyiadjis, P.I. Kattan,
*Advances in Damage Mechanics: Metals and Metal Matrix Composites With an Introduction to Fabric Tensors*(2nd edition), 742 p., (Elsevier, Oxford, ISBN: 0-08-044688-4, 2006)Google Scholar - G.Z. Voyiadjis, P.I. Kattan, A comparative study of damage variables in continuum damage mechanics. Int. J. Damage Mech.
**18**, 315–340 (2009)CrossRefGoogle Scholar - G.Z. Voyiadjis, P.I. Kattan, Mechanics of damage processes in series and in parallel: a conceptual framework. Acta Mech.
**223**, 1863–1878 (2012a)CrossRefMATHGoogle Scholar - G.Z. Voyiadjis, P.I. Kattan, A new class of damage variables in continuum damage mechanics. J. Eng. Mater. Technol.
**134**, 021016 (2012b)CrossRefGoogle Scholar - G.Z. Voyiadjis, P.I. Kattan, Healing and Super Healing in Continuum Damage Mechanics. Int. J. Damage Mech. 23(2), 245–260 (2014)Google Scholar
- G.Z. Voyiadjis, P.I. Kattan, How a Singularity Forms in Continuum Damage Mechanics. Mech. Res. Commun.
**55**, 86-88 (2014)Google Scholar - G.Z. Voyiadjis, P.I. Kattan, Introduction to the mechanics and design of undamageable materials. Int. J. Damage Mech.
**22**, 323–335 (2013c)Google Scholar - G.Z. Voyiadjis, P.I. Kattan, On the theory of elastic undamageable materials. J. Eng. Mater. Technol.
**135**, 021002 (2013d)Google Scholar - G.Z. Voyiadjis, N. Mozaffari, Nonlocal damage model using the phase field method: theory and applications. Int. J. Solids Struct.
**50**, 3136–3151 (2013)Google Scholar - G.Z. Voyiadjis, T. Park, Local and interfacial damage analysis of metal matrix composites. Int. J. Eng. Sci.
**33**, 1595–1621 (1995)CrossRefMATHGoogle Scholar - G.Z. Voyiadjis, T. Park, Anisotropic damage for the characterization of the onset of macro-crack initiation in metals. Int. J. Damage Mech.
**5**, 68–92 (1996)CrossRefGoogle Scholar - G. Voyiadjis, T. Park, Anisotropic damage effect tensors for the symmetrization of the effective stress tensor. J. Appl. Mech.
**64**, 106–110 (1997)CrossRefMATHGoogle Scholar - G.Z. Voyiadjis, Z.N. Taqieddin, P.I. Kattan, Theoretical formulation of a coupled elastic—plastic anisotropic damage model for concrete using the strain energy equivalence concept. Int. J. Damage Mech.
**18**, 603–638 (2009)CrossRefGoogle Scholar - G.Z. Voyiadjis, A. Shojaei, G. Li, P. Kattan, Continuum damage-healing mechanics with introduction to new healing variables. Int. J. Damage Mech.
**21**(3), 391–414 (2012)Google Scholar - G.Z. Voyiadjis, A. Shojaei, G. Li, A generalized coupled viscoplastic–viscodamage–viscohealing theory for glassy polymers. Int. J. Plast.
**28**, 21–45 (2012)CrossRefGoogle Scholar - S.-L. Wang, R.F. Sekerka, Algorithms for phase field computation of the dendritic operating state at large supercoolings. J. Comput. Phys.
**127**, 110–117 (1996)CrossRefMATHGoogle Scholar - J.A. Warren, W.J. Boettinger, Prediction of dendritic growth and microsegregation patterns in a binary alloy using the phase-field method. Acta Metall. Mater.
**43**, 689–703 (1995)CrossRefGoogle Scholar - A. Wheeler, B. Murray, R. Schaefer, Computation of dendrites using a phase field model. Phys. D Nonlinear Phenom.
**66**, 243–262 (1993)CrossRefMATHGoogle Scholar - S.R. White, N.R. Sottos, P.H. Geubelle, J.S. Moore, M.R. Kessler, S.R. Sriram, E.N. Brown, S. Viswanathan, Autonomic healing of polymer composites. Nature
**409**, 794–797 (2001)CrossRefGoogle Scholar - H.-L. Yu, C. Lu, K. Tieu, G.-Y. Deng, A numerical model for simulation of crack initiation around inclusion under tensile load. J. Comput. Theor. Nanosci.
**9**, 1745–1749 (2012)CrossRefGoogle Scholar - K. Yuan, J. Ju, New strain energy–based coupled elastoplastic damage-healing formulations accounting for effect of matric suction during earth-moving processes. J. Eng. Mech.
**139**, 188–199 (2012)CrossRefGoogle Scholar - F. Zaïri, M. Naït-Abdelaziz, J.-M. Gloaguen, J.-M. Lefebvre, A physically-based constitutive model for anisotropic damage in rubber-toughened glassy polymers during finite deformation. Int. J. Plast.
**27**, 25–51 (2011)CrossRefGoogle Scholar - M. Zako, N. Takano, Intelligent material systems using epoxy particles to repair microcracks and delamination damage in GFRP. J. Intell. Mater. Syst. Struct.
**10**, 836–841 (1999)CrossRefGoogle Scholar